2. WHAT IS HEAT TREATING?
Controlled Heating And Cooling of Metal to Change Its Properties
Through:Change in microstructure. Change in Chemistry or composition
Why Heat Treat?
• To improve Toughness
• To increase Hardness
• To increase Ductility
• To improve Machineability
• To refine Grain Structure
• To remove Residual Stresses
• To improve Wear Resistance
11. Full Annealing
The steel is heated above A3 (for hypo-eutectoid steels) & A1 (for hyper-eutectoid steels) →
(hold) → then the steel is furnace cooled to obtain Coarse Pearlite.
Coarse Pearlite has low (↓) Hardness but high (↑) Ductility.
For hyper-eutectoid steels the heating is not done above Acm to avoid a continuous network of
proeutectoid cementite along prior Austenite grain boundaries (presence of cementite along
grain boundaries provides easy path for crack propagation).
A microstructure with coarse
pearlite (i.e. pearlite having high
interlamellar spacing) is endowed
with such properties.
■ Makes a metal as soft as
■ Hypoeutectoid steels (less
than 0.83% carbon) are
heated above upper critical
temp., soaked and cooled
■ Hypereutecoid (above 0.83%)
are heated above lower
critical temp., soaked and
allowed to cool slowly.
13. ■ Process Annealing. Low
carbon steels may
harden through cold
working.They can be
heated to around 100
degrees below lower
critical temp., soaked
and allowed to cool in air.
■ Spheroidising. High
carbon steels may be
annealed just below the
lower critical temp. to
15. Recrystallization Annealing
Heat below A1 → Sufficient time → Recrystallization
During any cold working operation (say cold rolling), the material becomes harder
(due to work hardening), but loses its ductility. This implies that to continue
deformation the material needs to be recrystallized (wherein strain free grains
replace the ‘cold worked grains’).
Hence, recrystallization annealing is used as an intermediate step in (cold)
To achieve this the sample is heated below A1 and held there for sufficient time for
recrystallization to be completed.
16. Strain Hardening Due to Cold Drawing
New yield strength yi higher than initial yield strength, y0.
Reason strain hardening.
Strain Hardening due to Cold Drawing
Yield strength + hardness increased due to strain hardening,
but ductility decreased (material becomes more brittle).
19. Recovery, Recrystallization, and Grain Growth
Plastic deformation increases dislocation density +
changes grain size distribution
Therefore, stored strain energy (dislocation strain
fields + grain distortions)
External stress removed: most dislocations, grain
distortions and associated strain energy retained.
Restoration to state before cold-work by heat-
treatment: Recovery and Recrystallization,
followed by grain growth.
Heating increased diffusion
enhanced dislocation motion
decrease in dislocation density by annihilation,
formation of low-energy dislocation configurations
relieves internal strain energy
Some of the mechanisms of dislocation annihilation:
After recovery grains can still be strained. Strained grains
replaced upon heating by strain-free grains with
low density of dislocations.
Recrystallization: nucleation and growth of new grains
Driving force: difference in internal energy between
strained and unstrained
Grain growth short-range diffusion
Extent of recrystallization depends on temperature and time.
Recrystallization is slower in alloys
Recrystallization –effect of Cold work on temperature
Recrystallization temperature: temperature at which process is
complete in one hour. Typically 1/3 to 1/2 of melting temperature
(can be as high as 0.7 Tm in some alloys).
Recrystallization decreases as %CW is increased. Below "critical deformation",
recrystallization does not occur.
24. ■ To homogenize the structure which is dislocated
due to cold forming & semi hot & Hot forgings
Cold rolled Grain structure Annealed Grain structure
25. Stress Relief Annealing
Annihilation of dislocations,
Machining and cold working
Residual stresses → Heat below A1 → Recovery
Stress Relief Annealing
Due to various processes like quenching (differential cooling of surface and
interior), machining, phase transformations (like martensitic transformation),
welding, etc. the residual stresses develop in the sample.
Residual stress can lead to undesirable effects like warpage of the component.
The annealing is carried out just below A1 , wherein ‘recovery*’ processes are active
(Annihilation of dislocations, polygonization).
26. Spheroidization Annealing
This is a very specific heat treatment given to high carbon steel requiring extensive
machining prior to final hardening & tempering.
The main purpose of the treatment is to increase the ductility of the sample.
Like stress relief annealing the treatment is done just below A1.
Long time heating leads cementite plates to form cementite spheroids. The driving
force for this (microstructural) transformation is the reduction in interfacial energy.
The process might be more accurately described as a homogenizing or
grain-refining treatment. Within any piece of steel, the composition is
usually not uniform throughout.
That is, one area may have more carbon than the area adjacent to it.
These cornpositional differences affect the way in which the steel will
respond to heat treatment.
Because of characteristics inherent in cast steel, the normalizing
treatment is more frequently applied to ingots prior to working, and to
steel castings and forgings prior to hardening.
28. ■ Normalising. Internal stresses caused by rolling and rolling or forging
are removed. Steels are heated above upper critical temp., soaked
and cooled in air. The cooling rate is faster than annealing giving a
smaller grain structure.
■ Stress relieving. The component is reheated and held at temperature
for a period of time and cooled slowly.
29. To aid machinability ,to eliminate the nonconformities
present in microstructure such as banding – Normalising is
Refine grain structure prior to hardening
To harden the steel slightly
To reduce segregation in casting or forgings
The sample is heat above A3 | Acm to complete Austenization.
The sample is then air cooled to obtain Fine pearlite.
Fine pearlite has a reasonably good hardness and ductility.
In hypo-eutectoid steels normalizing is done 50C above the annealing temperature.
In hyper-eutectoid steels normalizing done above Acm → due to faster cooling
cementite does not form a continuous film along GB.
The list of uses of normalizing are listed below.
Heat above A3 | Acm → Austenization → Quench (higher than critical cooling rate)
The sample is heated above A3 | Acm to cause Austenization.
The sample is then quenched at a cooling rate higher than the critical cooling rate
(i.e. to avoid the nose of the CCT diagram).
The quenching process produces residual strains (thermal, phase transformation).
The transformation to Martensite is usually not complete and the sample will have
some retained Austenite.
The Martensite produced is hard and brittle and tempering operation usually follows
hardening. This gives a good combination of strength and toughness.
■ Medium and High carbon steels (0.4 – 1.2%) can be heated
until red hot and then quenched in water producing a very
hard and brittle metal. At 723 degrees, the BCC ferrite
changes into Austenite with a FCC structure.
■ Thermal stresses during heating should be avoided.
■ In every heat treatment, the heating process is named
ramping. The ramping for hardening should be made in
■ preheating temperatures are 600–650°C (1100–
■ 1200°F) and 800–850°C (1450–1560°F).
■ In the case of high speed steel, the holding time will be
shorter when the hardening temperature is over
■ If the holding time is prolonged, microstructural
problems like grain growth can arise.
■ To get the best microstructure and tool performance the
quenching rate should be rapid. To minimize distortion,
a slow quenching rate is recommended.
38. Through hardening of the sample
Schematic showing variation
in cooling rate from surface
to interior leading to
39. Typical hardness test survey made along a
diameter of a quenched cylinder
The surface of is affected by the quenching medium and experiences the best possible
The interior of the sample is cooled by conduction through the (hot) sample and hence
experiences a lower cooling rate.
This implies that different parts of the same sample follow different cooling curves on a
CCT diagram and give rise to different microstructures.
This gives to a varying hardness from centre to circumference. Critical diameter (dc) is that
diameter, which can be through hardened (i.e. we obtain 50% Martensite and 50% pearlite at
the centre of the sample).
40. Jominy hardenability test Variation of hardness along a Jominy bar
(schematic for eutectoid steel)
Schematic of Jominy End Quench Test
41. How to increase hardenability?
Hardenability should not be confused with the ability to obtain high hardness. A material
with low hardenability may have a higher surface hardness compared to another sample
with higher hardenability.
A material with a high hardenability can be cooled relatively slowly to produce 50%
martensite (& 50% pearlite). A material with a high hardenability has the ‘nose’ of the CCT
curve ‘far’ to the right (i.e. at higher times). Such a material can be through hardened easily.
TTT diagram of low alloy steel (0.42%
C, 0.78% Mn, 1.79% Ni, 0.80% Cr,
U.S.S. Carilloy Steels, United States
Steel Corporation, Pittsburgh, 1948)
Hardenability of plain carbon steel can increased by
alloying with most elements (it is to be noted that this is
an added advantage as alloying is usually done to
improve other properties).
However, alloying gives two separate ‘C-curves’ for
Pearlitic and Bainitic transformations (e.g. figure to the
This implies that the ‘nose’ of the Bainitic
transformation has to be avoided to get complete
Martensite on quenching.
42. ■ SUB-ZERO TREATMENT
■ Retained austenite in a tool can transform into
martensite during service.
■ This will lead to local distortion and embrittlement of
the tool due to the presence of untempered martensite.
■ Therefore the requirement of maximum dimensional
stability in service has an implied demand for very low
or no retained austenite content.
■ This can be achieved by using sub-zero treatment after
■ The most commonly used are about -80°C (-110°F)
■ and -196°C (-320°F).
■ This, in turn, will result in a hardness increase of up to
■ The material should be tempered immediately after
quenching to avoid cracks .
■ Quenching should be stopped at a temperature of 50–
70°C (120–160°F) and tempering should be done at
■ If this is not possible, the material must be kept warm,
■ e.g. in a special “hot cabinet” awaiting tempering.
■ Two tempers are generally recommended for tool steel,
except in the cases of large cross-sections, parts with
■ A second tempering gives the material optimum
toughness at the chosen hardness level
■ To remove some of the brittleness from hardened steels,
tempering is used. The metal is heated to the range of 220-
300 degrees and cooled.
■ Tempering colours are an indicator of temperature on
polished metals. Colours range from yellow to brown to violet
A sample with martensitic microstructure is hard but brittle. Hence after quenching
the sample (or component) is tempered. Maternsite being a metastable phase
decomposes to ferrite and cementite on heating (providing thermal activation).
Tempering is carried out just below the eutectoid temperature (heat → wait→ slow
In reality the microstructural changes which take place during tempering are very
The time temperature cycle for tempering is chosen so as to optimize strength and
E.g. tool steel has a as quenched hardness of Rc65, which is tempered to get a
hardness of Rc45-55.
BCT Temper )(Ce)()(' 3
Pearlite + Bainite
0.1 1 10 102 103 104
t (s) →
MARTEMPERING & AUSTEMPERING
These processes are developed to avoid residual stresses generated in quenching.
In both these processes Austenized steel is quenched above Ms (to a temp T1) for
homogenization of temperature across the sample.
In Martempering the steel is then quenched and the entire sample transforms
simultaneously to martensite. This is followed by tempering.
In Austempering instead of quenching the sample, it is held at T1 for it to transform